Slow relaxation of magnetization in unprecedented Cu‒Ln-Rad hetero-tri-spin chains constructed from multidentate nitronyl nitroxide
Sun, Juan; Sun, Zan; Wang, Kang; Xi, Lu; Ma, Yue; Li, Licun; Journal of Materials Chemistry C 7 (2019) 9057–; doi:10.1039/C9TC02410G

data_7237867
_publ_section_title
;
 Slow relaxation of magnetization in unprecedented Cu--Ln-Rad
 hetero-tri-spin chains constructed from multidentate nitronyl nitroxide
;
_journal_issue                   29
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              9057
_journal_paper_doi               10.1039/C9TC02410G
_journal_volume                  7
_journal_year                    2019
_chemical_formula_sum            'C58 H32 Cu2 F42 N4 O17 Tb'
_chemical_formula_weight         2140.91
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2019-06-23 deposited with the CCDC.	2019-06-27 downloaded from the CCDC.
;
_cell_angle_alpha                75.1108(14)
_cell_angle_beta                 85.3367(13)
_cell_angle_gamma                86.9439(14)
_cell_formula_units_Z            2
_cell_length_a                   12.1727(2)
_cell_length_b                   16.4693(3)
_cell_length_c                   20.6836(3)
_cell_measurement_reflns_used    32684
_cell_measurement_temperature    120
_cell_measurement_theta_max      74.1230
_cell_measurement_theta_min      3.9410
_cell_volume                     3991.81(12)
_computing_cell_refinement       'CrysAlisPro 1.171.39.33c (Rigaku OD, 2017)'
_computing_data_collection       'CrysAlisPro 1.171.39.33c (Rigaku OD, 2017)'
_computing_data_reduction        'CrysAlisPro 1.171.39.33c (Rigaku OD, 2017)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'XS (Sheldrick, 2008)'
_diffrn_ambient_temperature      120
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0281
_diffrn_reflns_av_unetI/netI     0.0268
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            43451
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.010
_diffrn_reflns_theta_max         25.010
_diffrn_reflns_theta_min         1.679
_exptl_absorpt_coefficient_mu    1.565
_exptl_absorpt_correction_T_max  0.731
_exptl_absorpt_correction_T_min  0.632
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            purple-green
_exptl_crystal_density_diffrn    1.781
_exptl_crystal_description       block
_exptl_crystal_F_000             2090
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.2
_refine_diff_density_max         2.556
_refine_diff_density_min         -1.627
_refine_diff_density_rms         0.171
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.100
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1198
_refine_ls_number_reflns         14026
_refine_ls_number_restraints     119
_refine_ls_restrained_S_all      1.118
_refine_ls_R_factor_all          0.0857
_refine_ls_R_factor_gt           0.0838
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1060P)^2^+42.0819P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2251
_refine_ls_wR_factor_ref         0.2265
_reflns_Friedel_coverage         0.000
_reflns_number_gt                13453
_reflns_number_total             14026
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9tc02410g2.cif
_cod_data_source_block           12
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_database_code               7237867
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              74136
_shelx_fab_checksum              90261